Materials 2014, 7, 5711-5734; doi:10.3390/ma7085711
materials ISSN 1996-1944
The Inhibition of Aluminum Corrosion in Sulfuric Acid by Poly(1-vinyl-3-alkyl-imidazolium Hexafluorophosphate)
Paulina Arellanes-Lozada 1, Octavio Olivares-Xometl 2,*, Diego Guzmn-Lucero 3, Natalya V. Likhanova 3, Marco A. Domnguez-Aguilar 3, Irina V. Lijanova 4 and Elsa Arce-Estrada 1
1 Instituto Politcnico Nacional, ESIQIE, Departamento de Metalurgia y Materiales, Av. Instituto Politcnico Nacional S/N, Col. Lindavista, Mxico D.F. 07300, Mexico; E-Mails: email@example.com (P.A.-L.); firstname.lastname@example.org (E.A.-E.)
2 Facultad de Ingeniera Qumica, Benemrita Universidad Autnoma de Puebla, Av. San Claudio, Ciudad Universitaria. Col. San Manuel, Puebla, Puebla 72570, Mexico
3 Instituto Mexicano del Petrleo, Programa de Investigacin y Posgrado, Eje Central Lzaro Crdenas No. 152, Col. San Bartolo Atepehuacn, Mxico D.F. 07730, Mexico; E-Mails: email@example.com (D.G.-L.); firstname.lastname@example.org (N.V.L.); email@example.com (M.A.D.-A.)
4 Instituto Politcnico Nacional, CIITEC, Cerrada Cecati S/N, Colonia Santa Catarina, Azcapotzalco, Mxico D.F. 02250, Mexico; E-Mail: firstname.lastname@example.org
* Author to whom correspondence should be addressed; E-Mail: email@example.com or firstname.lastname@example.org; Tel.: +52-559-175-8382.
Received: 8 May 2014; in revised form: 23 July 2014 / Accepted: 29 July 2014 / Published: 7 August 2014
Abstract: Compounds of poly(ionic liquid)s (PILs), derived from imidazole with different alkylic chain lengths located in the third position of the imidazolium ring (poly(1-vinyl-3-dodecyl-imidazolium) (PImC12), poly(1-vinyl-3-octylimidazolium) (PImC8) and poly(1-vinyl-3-butylimidazolium) (PImC4) hexafluorophosphate) were synthesized. These compounds were tested as corrosion inhibitors on aluminum alloy AA6061 in diluted sulfuric acid (0.11 M H2SO4) by weight loss tests, polarization resistance measurements and inductively coupled plasma optical emission spectroscopy. Langmuirs isotherms suggested film formation on bare alloy while standard free energy indicated inhibition by a physisorption process. However, compound efficiencies as inhibitors ranked low (PImC12 > PImC8 > PImC4) to reach 61% for PImC12 in highly diluted acidic solution. Apparently, the high mobility of sulfates favored their adsorption in comparison to PILs. The surface film displayed general corrosion, and pitting occurred as a consequence of
Materials 2014, 7 5712
PILs partial inhibition along with a continuous dissolution of defective patchy film on formation. A slight improvement in efficiency was displayed by compounds having high molecular weight and a long alkyl chain, as a consequence of steric hindrance and PIL interactions.
Keywords: alloys; surfaces; corrosion test; electrochemical techniques; adsorption
Aluminum and its alloys find a wide variety of technological applications owing to the balanced combination of physical, mechanical and chemical properties, such as electrical and thermal conductivities, low density, high ductility, stability for surface treatments, good corrosion resistance, easiness of recycling and functional advantages of extruded and cast semi-products . The addition of elements, such as copper, lithium, manganese, magnesium, silicon and zinc, allows aluminum to achieve a long range of bulk properties; likewise, minor additions provide an improvement in specific properties .
Aluminum generally exhibits passive behavior in aqueous solution due to the formation of a strong and compact adherent passive oxide film on the surface, which affects corrosion susceptibility. The adhesive passivating surface oxide film is amphoteric, and consequently, the metal is readily dissolved when exposed to aggressive acidic and alkaline solutions. In fact, the corrosion of metallic materials in acidic solution causes considerable costs [5,6]. In near-neutral solutions, the solubility of oxides will be much lower than in acidic solutions, and the extent of dissolution will tend to be smaller [7,8].
The presence of aggressive ions (chlorides, fluorides) attacks the oxide film locally, and certain elements (Ga, Tl, In, Sn, Pb, Fe) are incorporated into it, which may have a deleterious effect. Most commercial alloys contain several types of intermetallic phases, where aluminum corrosion occurred essentially as a micro-galvanic process between these secondary phases and the matrix alloy . Sulfuric acid solutions are widely used for aluminum anodizing operations. Additionally, aluminum and its alloys are designated for industrial applications to manage a large variety of acid and alkaline solutions, but once dissolved, corrosion of the naturally-formed film can only be controlled by efficient inhibitors.
The use of chemicals as corrosion inhibitors (CIs) is one of the most popular and efficient methods to protect metals; this is a convenient and relatively inexpensive method to achieve this goal . Organic compounds are commonly used as CIs in industry, such as those having electrons in structure and containing nitrogen, sulfur, phosphorus and oxygen atoms, through which they are adsorbed on the metal surface . The adsorption is influenced by the electronic structure of the inhibiting molecules  and also by steric factors, aromaticity, electron density at the donor atoms and the presence of functional groups . The use of polymers as CIs has attracted considerable attention due to their inherent stability and cost effectiveness . Several families of homopolymers have been widely studied: polyacrylamide, polyvinyl pyrrolidone, polyacrylic acid and polyethyleneimine, It is known that polymers are strongly adsorbed on the surface, though giving lower toxicity than their analogues; hence, it is expected that polymers will be better corrosion inhibitors than
Materials 2014, 7 5713
the corresponding monomers [29,30]. Polymers may provide some advantages in comparison to other organic molecules: They provide a large single chain that displaces water molecules from metallic surface and makes inhibition more favorable. The presence of multiple bonding sites on the metallic surface makes polymer desorption a slow process . Polymers form complexes with metal ions, and these complexes occupy a larger surface area, thereby blanketing the surface and protecting metal from the corrosive agents contained in solution .
In the present work, the effect of three poly(ionic liquid)s (PILs) (poly(1-vinyl-3-dodecylimidazolium hexafluorophosphate), poly(1-vinyl-3-octylimidazolium hexafluorophosphate) and poly(1-vinyl-3-butylimidazolium hexafluorophosphate)) were tested as CIs in a concentration range within 10 to 100 mgL1 (ppm) in aqueous sulfuric acid to prevent the corrosion of aluminum alloy AA6061. Weight loss tests, potentiodynamic polarization and surface analysis were used to support the proposed mechanism of inhibition. As not many polymers are considered as good corrosion inhibitors for non-ferrous metals and its alloys since surface adsorption is not always a straightforward process, it was decided to synthesize polymers based on ILs, as they possess a polymeric structure with surfactant components having positive and negative charges along with a hydrophobic chain
2. Experimental Section
2.1. Synthesis and Characterization of PILs
PILs were synthesized and characterized by 1H and 13C NMR and IR spectroscopies. Melting points were measured in a Fisher Scientific apparatus equipped with a 300 C thermometer. FT-IR spectra were registered on a Nicolet FT-IR 5DX FT spectrophotometer as KBr discs. 1H NMR (300 MHz) and 13C NMR (75.4 MHz) spectra were obtained in a JEOL Eclipse-300 equipment using TMS as the internal standard. DMSO-d6 was used as solvent for PImC8 and PImC4, and CDCl3 for PImC12, in each case, dissolution was performed at room temperature. The gel permeation chromatography system was performed in a Waters 2410 refractive index detector with a 3 PL gel 10-m mixed-B columns to determine molecular weights. The GPC was calibrated with a polystyrene standard with tetrahydrofuran as the eluent.
The monomers of 1-vinyl-3-alkylimidazolium hexafluorophosphate were obtained according to the reported procedure , while the polymerization of 1-vinyl-3-alkylimidazolium hexafluorophosphates was carried out by free radical polymerization in solution using 2,2-azo-bis(isobutyronitrile) as described elsewhere  to obtain white solid products in a 97% yield. Table 1 shows the common chemical name and abbreviation for the compounds used in the present study. The polymerization was proven by the disappearance of the peaks corresponding to the vinyl group in the 1H NMR at 5.44, 5.96 and 7.26 ppm, 13C NMR at 108.6 and 119.1 ppm  and the appearance of new peaks corresponding to the polyvinyl group at around 3.24 and 2.2 ppm in 1H NMR (Table 2).
Materials 2014, 7 5714
Table 1. The poly(ionic liquid)s (PILs) tested as corrosion inhibitors.
Abbreviation Name Structure MW (g/mol) DP IR, cm1
60,500 148 3,168, 2,934, 2,879, 1,553, 1,475, 837,
51,400 145 3,168, 2,931, 2,859, 1,554, 1,469, 1,164,
835, 736, 557
32,300 108 3,166, 2,969, 2,881, 1,552, 1,471, 1,162,
836, 738, 557
Table 2. NMR characterization of synthesized PILs.
1H NMR, ppm 13C NMR, ppm